Download presentation

Presentation is loading. Please wait.

Published byIsabella Tarte Modified about 1 year ago

1
1 Texture Components and Euler Angles: part 1 June 2007 L3 from , Advanced Characterization & Microstructural Analysis, A.D. (Tony) Rollett

2
2 Lecture Objectives Show how to convert from a description of a crystal orientation based on Miller indices to matrices to Euler angles Give examples of standard named components and their associated Euler angles The overall aim is to be able to describe a texture component by a single point (in some set of coordinates such as Euler angles) instead of needing to draw the crystal embedded in a reference frame Part 1 will provide a mainly qualitative, pictorial approach to illustrate the physical meaning of Euler angles and “orientations”; part 2 will provide more mathematical detail Obj/notation AxisTransformation Matrix EulerAngles Components

3
3 Miller Index Definition of a Crystal Orientation We use a set of three orthogonal directions as the reference frame. Mathematicians set up a set of unit vectors called e 1 e 2 and e 3. In many cases we use the names Rolling Direction (RD) // e 1, Transverse Direction (TD) // e 2, and Normal Direction (ND) // e 3. We then identify a crystal (or plane normal) parallel to 3 rd axis (ND) and a crystal direction parallel to the 1 st axis (RD), written as (hkl)[uvw].

4
4 (Bunge) Euler Angle Definition Obj/notation AxisTransformation Matrix EulerAngles Components The three reference axes are labeled as X, Y & Z; also commonly known as ND, RD, and TD. The three crystal axes are labeled as X’, Y’ & Z’ ; also commonly known as [100], [010] & [001] in cubic crystals.

5
5 Euler Angles, Animated [010] [100] [001] Crystal e 1 =X sample =RD e 2 =Y sample =TD e 3 =Z sample =ND Sample Axes RD TD e” 2 e” 3 =e” 1 2 nd position y crystal =e 2 ’’’ x crystal =e 1 ’’’ z crystal =e 3 ’’’ = 3 rd position (final) e’ 1 e’ 2 e’ 3 = 1 st position

6
6 Cube Texture (100)[001]: cube-on-face Observed in recrystallization of fcc metals The 001 orientations are parallel to the three ND, RD, and TD directions. Obj/notation AxisTransformation Matrix EulerAngles Components

7
7 Sharp Texture (Recrystallization) Look at the (001) pole figures for this type of texture: maxima correspond to {100} poles in the standard stereographic projection. Obj/notation AxisTransformation Matrix EulerAngles Components

8
8 Euler angles of Cube component The Euler angles for this component are simple, and yet not so simple! The crystal axes align exactly with the specimen axes, therefore all three angles are exactly zero: ( 1, , 2 ) = (0°, 0°, 0°). As an introduction to the effects of crystal symmetry: consider aligning [100]//TD, [010]//-RD, [001]//ND. This is evidently still the cube orientation, but the Euler angles are ( 1, , 2 ) = (90°,0°,0°)! Obj/notation AxisTransformation Matrix EulerAngles Components

9
9 {011} : the Goss Component This type of texture is known as Goss Texture and occurs as a Recrystallization texture for FCC materials such as Brass, … In this case the (011) plane is oriented towards the ND and the [001] inside the (011) plane is along the RD. RD ND TD (110) [100] Obj/notation AxisTransformation Matrix EulerAngles Components

10
10 {011} : cube-on-edge In the 011 pole figure, one of the poles is oriented parallel to the ND (center of the pole figure) but the other ones will be at 60° or 90° angles but tilted 45° from the RD! (Homework: draw the (111) pole figure) RD ND TD (110) [100] {110}

11
11 Euler angles of Goss component The Euler angles for this component are simple, and yet other variants exist, just as for the cube component. Only one rotation of 45° is needed to rotate the crystal from the reference position (i.e. the cube component); this happens to be accomplished with the 2nd Euler angle. ( 1, , 2 ) = (0°,45°,0°). Other variants will be shown when symmetry is discussed. Obj/notation AxisTransformation Matrix EulerAngles Components

12
12 Brass component This type of texture is known as Brass Texture and occurs as a rolling texture component for materials such as Brass, Silver, and Stainless steel. Obj/notation AxisTransformation Matrix EulerAngles Components

13
13 Brass component, contd. (100)(111)(110) Obj/notation AxisTransformation Matrix EulerAngles Components The associated (110) pole figure is very similar to the Goss texture pole figure except that it is rotated about the ND. In this example, the crystal has been rotated in only one sense (anticlockwise).

14
14 {110} Brass component Think of rotating the Goss component around the ND. In this example, the xtal has been rotated in both senses (two variants).

15
15 Brass component: Euler angles The brass component is convenient because we can think about performing two successive rotations: 1st about the ND, 2nd about the new position of the [100] axis. 1st rotation is 35° about the ND; 2nd rotation is 45° about the [100]. ( 1, , 2 ) = (35°,45°,0°). Obj/notation AxisTransformation Matrix EulerAngles Components

16
16 Obj/notation AxisTransformation Matrix EulerAngles Components

17
17 Meaning of “Variants” The existence of variants of a given texture component is a consequence of (statistical) sample symmetry. If one permutes the Miller indices for a given component (for cubics, one can change the sign and order, but not the set of digits), then different values of the Euler angles are found for each permutation. If a pole figure is plotted of all the variants, one observes a number of physically distinct orientations, which are related to each other by symmetry operators (diads, typically) fixed in the sample frame of reference. Each physically distinct orientation is a “variant”. The number of variants listed depends on the choice of size of Euler space (typically 90x90x90°) and the alignment of the component with respect to the sample symmetry.

18
18 Euler Angle Conventions An inconvenient fact is that the definition of Euler angles that we have given so far is not unique. Many other variants not only exist but have names and are in regular use! The differences between the conventions lie in the choice of the rotation axes (generally only the second axis) and the sense of rotation. Some of the commonly used conventions are Bunge, Roe and Kocks (in approximate order of decreasing popularity).

19
19 Kocks Euler Angles: Ship Analogy Analogy: position and the heading of a boat with respect to the globe. Latitude ( ) and longitude ( ) describe the position of the boat; third angle describes the heading ( ) of the boat relative to the line of longitude that connects the boat to the North Pole. Kocks vs. Bunge angles: to be explained later! Obj/notation AxisTransformation Matrix EulerAngles Components

20
20 Meaning of Euler angles In the Bunge convention, the first two angles, 1 and , tell you the position of the [001] crystal direction relative to the specimen axes. Think of rotating the crystal about the ND (1st angle, 1 ); then rotate the crystal out of the plane (about the [100] axis, ); Finally, the 3 rd angle ( 2 ) tells you how much to rotate the crystal about [001]. Obj/notation AxisTransformation Matrix EulerAngles Components

21
21 Euler Angle Definitions Bunge and Canova are inverse to one another Kocks and Roe differ by sign of third angle Bunge rotates about x’, Kocks about y’ (2nd angle) Obj/notation AxisTransformation Matrix EulerAngles Components Kocks

22
22 Conversions Obj/notation AxisTransformation Matrix EulerAngles Components

23
23 Complete orientations in the Pole Figure 11 11 22 22 Note the loss of information in a diffraction experiment if each set of poles from a single component cannot be related to one another. ( 1, , 2 ) ~ (30°,70°,40°). Obj/notation AxisTransformation Matrix EulerAngles Components

24
24 Complete orientations in the Inverse Pole Figure Think of yourself as an observer standing on the crystal axes, and measuring where the sample axes lie in relation to the crystal axes. Obj/notation AxisTransformation Matrix EulerAngles Components

25
25 Summary Conversion between different forms of description of texture components described. Physical picture of the meaning of Euler angles as rotations of a crystal given. Miller indices are descriptive, but matrices are useful for computation, and Euler angles are useful for mapping out textures (to be discussed).

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google